Resin cements create a high bond between the tooth and ceramic surfaces, thus making it impossible to remove the restoration in one piece. The aims of this study were to evaluate (i) the efficiency of an Er:YAG laser for debonding, and (ii) the changes in the rebonding strength values of all-ceramic veneers, which were removed after laser application. A tooth reduction of 120 extracted human maxillary central incisors was made to provide two different bonding surfaces (60 enamel and 60 dentin). Sixty leucite and 60 lithium disilicate discs (1-mm thickness, 5-mm diameter) were cemented to prepared surfaces with a dual-cure resin cement. Each group was divided into two subgroups (n = 15): control and laser-irradiated. Er:YAG laser (2940 nm) was applied for 9 s at 3 W power (10 Hz, 300 mJ) with 100 μs pulse duration. Shear bond strength (SBS) test was made with a universal testing machine. After the tested laser-irradiated specimens had been rebonded, the SBS test was performed again and rebonding strengths were measured. The statistical evaluations were performed by using repeated measures one-way ANOVA and post hoc Bonferroni tests (p < 0.05). Significant differences were found between the control and laser-irradiated groups (p < 0.001). While the required SBS values for control groups were between 30.04 and 24.66 MPa, the values for laser-irradiated groups were between 6.60 and 4.09 MPa. There was no significant difference between the control and rebonded groups. Er:YAG laser-irradiation is an effective method for removing all-ceramic restorations without affecting the rebonding strength.
This is a preview of subscription content, access via your institution.
Buy single article
Instant access to the full article PDF.
Tax calculation will be finalised during checkout.
Subscribe to journal
Immediate online access to all issues from 2019. Subscription will auto renew annually.
Tax calculation will be finalised during checkout.
Fabbri G, Zarone F, Dellificorelli G, Cannistraro G, De Lorenzi M, Mosca A, Sorrentino R (2014) Clinical evaluation of 860 anterior and posterior lithium disilicate restorations: retrospective study with a mean follow-up of 3 years and a maximum observational period of 6 years. Int J Periodontics Restorative Dent 34:165–177
Gehrt M, Wolfart S, Rafai N, Reich S, Edelhoff D (2013) Clinical results of lithium-disilicate crowns after up to 9 years of service. Clin Oral Investig 17:275–284
Gracis S, Thompson VP, Ferencz JL, Silva NS, Bonfante EA (2015) New Classication system for all-ceramic and ceramic-like restorative materials. Int J Prosthodont 28:227–235
Peumans M, Van Meerbeek B, Lambrechts P, Vanherle G (2000) Porcelain veneers: a review of the literature. J Dent 28:163–177
Oztoprak MO, Tozlu M, Iseri U, Ulkur F, Arun T (2012) Effects of different application durations of scanning laser method on debonding strength of laminate veneers. Lasers Med Sci 27:713–716
Van As G (2013) Using the erbium laser to remove porcelain veneers in 60 seconds. J Cosmetic Dent 28:20–34
Kellesarian SV, Malignaggi VR, Aldosary KM (2017) Laser assisted removal of all ceramic fixed dental prostheses: a comprehensive review. J Esthet Restor Dent 30:216–222. https://doi.org/10.1111/jerd.12360
Whitehead SA, Aya A, Macfarlane TV, Watts DC, Wilson NH (2000) Removal of porcelain veneers aided by a fluorescing luting cement. J Esthet Dent 12:38–45
Rechmann P, Buu NC, Rechmann BM, Finzen FC (2014) Laser all-ceramic crown removal-a laboratory proof-of-principle study-phase 2 crown debonding time. Lasers Surg Med 46:636–643
Sari T, Tuncel I, Usumez A, Gutknecht N (2014) Transmission of Er: YAG laser through different dental ceramics. Photomed Laser Surg 32:37–41
Strobl K, Bahns TL, Willham L, Bishara SE, Stwalley WC (1992) Laser-aided debond- ing of orthodontic ceramic brackets. Am J Orthod Dentofac Orthop 101:152–158
Ma T, Marangoni RD, Flint W (1997) In vitro comparison of debonding force and intrapulpal temperature changes during ceramic orthodontic bracket removal using a carbon dioxide laser. Am J Orthod Dentofac Orthop 111:203–210
Tocchio RM, Williams PT, Mayer FJ, Standing KG (1993) Laser debonding of ceramic orthodontic brackets. Am J Orthod Dentofac Orthop 103:155–162
Feldon PJ, Murray PE, Burch JJ, Meister M, Freedman MA (2010) Diode laser debonding of ceramic brackets. Am J Orthod Dentofac Orthop 138:458–462
Sarp AS, Gulsoy M (2011) Ceramic bracket debonding with ytterbium fiber laser. Lasers Med Sci 26:577–584
Mundethu AR, Gutknecht N, Franzen R (2014) Rapid debonding of polycrystalline ceramic orthodontic brackets with an Er:YAG laser: an in vitro study. Lasers Med Sci 29:1551–1556
Morford CK, Buu NC, Rechmann BM, Finzen FC, Sharma AB, Rechmann P (2011) Er:YAG laser debonding of porcelain veneers. Lasers Surg Med 43:965–974
Albalkhi M, Swed E, Hamadah O (2018) Efficiency of Er:YAG laser in debonding of porcelain laminate veneers by contact and non-contact laser application modes (in vitro study). J Esthet Restor Dent 30:223–228
Bulut AC, Atsu SS (2017) The effect of repeated bonding on the shear bond strength of different resin cements to enamel and dentin. J Adv Prosthodont 9:57–66
Gurney ML, Sharples SD, Phillips WB, Lee DJ (2016) Using an Er, Cr: YSGG laser to remove lithium disilicate restorations: a pilot study. J Prosthet Dent 115:90–94
Iseri U, Oztoprak MO, Ozkurt Z (2014) Effect of Er:YAG laser on debonding strength of laminate veneers. Eur J Dent 8:58–62
Broome PJ (2007) Utilization of an Er, Cr:YSGG laser for the removal of all-ceramic restorations. Pract Proced Aesthet Dent 19:23–25
Cranska JP (2015) Laser removal of all-ceramic restorations. Solving a difficult clinical challenge. Dent Today 34:110–113
Cranska JP (2013) Removing all-ceramic restorations with lasers. Dent Today 32(101–102):104
Spath A, Smith C (2017) Removal of modern ceramics. Compend Contin Educ Dent 38:326–233
van As G (2012) Laser removal of porcelain veneers. Dent Today 31:84 86, 88-9
Kursoglu P, Gursoy H (2013) Removal of fractured laminate veneers with Er:YAG laser: report of two cases. Photomed Laser Surg 31:41–43
Tehranchi A, Fekrazad R, Zafar M, Eslami B, Kalhori KM, Gutknecht N (2011) Evaluation of the effects of CO2 laser on debonding of orthodontics porcelain brackets vs. the conventional method. Lasers Med Sci 26:563–567
Elkamhawy NH, Elkadi AS, Alabbassy FH (2016) Shear bond strength of ceramic laminate veneers to enamel and enamel-dentine complex bonded with different adhesive luting systems. Alex Dent J 41:131–137
Mak YF, Lai SC, Cheung GS, Chan AW, Tay FR, Pashley DH (2002) Micro-tensile bond testing of resin cements to dentine and an indirect resin composite. Dent Mater 18:609–621
Zhang Y, Rocca J, Fornaini C, Zhen Y, Zhao Z, Merigo E (2018) Er:YAG laser debonding of porcelain laminate veneers. Preprints 2018060086. https://doi.org/10.20944/preprints201806.0086.v1
Rechmann P, Buu NC, Rechmann BM, Finzen FC (2015) Laser all-ceramic crown removal and pulpal temperature–a laboratory proof-of- principle study. Lasers Med Sci 30:2087–2093
Nalbantgil D, Oztoprak MO, Tozlu M, Arun T (2011) Effects of different application durations of Er:YAG laser on intrapulpal temperature change during debonding. Lasers Med Sci 26:735–740
Ozturk E, Bolay S, Hickel R, Ilie N (2013) Shear bond strength of porcelain laminate veneers to enamel, dentine and enamel–dentine complex bonded with different adhesive luting systems. J Dent 41:97–105
Bishara SE, Von Wald L, Laffoon JF, Warren JJ (2000) The effect of repeated bonding on the shear bond strength of a composite resin orthodontic adhesive. Angle Orthod 70:435–441
Montasser MA, Drummond JL, Evans CA (2008) Rebonding of orthodontic brackets. Part I, a laboratory and clinical study. Angle Orthod 78:531–536
Koodaryan R, Hafezegoran A, Khakpour Maleki A (2017) The effect of resin cement type and cleaning method on the shear bond strength of resin cements for recementing restorations. J Adv Prosthodont 9:110–117
Sol E, Espasa E, Boj JR, Canalda C (2000) Effect of different prophylaxis methods on sealant adhesion. J Clin Pediatr Dent 24:211–214
Blixt M, Adamczak E, Lindén LA, Odén A, Arvidson K (2000) Bonding to densely sintered alumina surfaces: effect of sandblasting and silica coating on shear bond strength of luting cements. Int J Prosthodont 13:221–226
Calamia JR, Calamia CS (2007) Porcelain laminate veneers: reasons for 25 years of success. Dent Clin N Am 51:399–417
Chen TM, Brauer GM (1982) Solvent effects on bonding organo-silane to silica surfaces. J Dent Res 61:1439–1443
Román-Rodríguez JL, Alonso-Pérez-Barquero J, Bruguera-Álvarez A, Agustín-Panadero R, Fons-Font A (2015) Cleaning and retreatment protocol for a debonded ceramic restoration. J Clin Exp Dent 7:e60–e62. https://doi.org/10.4317/jced.51891
St Germain HA Jr, St Germain TH (2015) Shear bond strength of porcelain veneers rebonded to enamel. Oper Dent 40:E112–E121. https://doi.org/10.2341/14-123-L
Azzeh E, Feldon PJ (2003) Laser debonding of ceramic brackets: a comprehensive review. Am J Orthod Dentofac Orthop 123:79–83
Gozneli R, Kazazoglu E, Ozkan Y (2014) Flexural properties of leucite and lithium disilicate ceramic materials after repeated firings. J Dent Sci 9:144–150
This study was supported in part by a research grant from the Scientific Research Projects Committee of Marmara University, Istanbul (Project no. SAG-C-DUP-170118-0004).
Conflict of interest
The authors declare that they have no conflicts of interest.
This article does not contain any studies with human participants or animals performed by any of the authors.
This article only contains a study with test samples prepared by using extracted human maxillary central incisors that were previously extracted for periodontal reasons.
Although no human participants or animals performed, this study was approved by the university human research ethics committee and all procedures performed in studies (involving human participants) were in accordance with the ethical standards of the institutional and/or national research committee and with the 1964 Helsinki declaration and its later amendments or comparable ethical standards.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Karagoz-Yildirak, M., Gozneli, R. Evaluation of rebonding strengths of leucite and lithium disilicate veneers debonded with an Er:YAG laser. Lasers Med Sci 35, 853–860 (2020). https://doi.org/10.1007/s10103-019-02872-8
- Er:YAG laser
- Shear bond strength